Journal of Environmental Sciences 21(2009) 539–544
Kinetic adsorption of application of carbon nanotubes for Pb(II) removal from aqueous solution Nassereldeen A Kabbashi1,2,∗, Muataz A Atieh3 , Abdullah Al-Mamun1 , Mohamed E S Mirghami1 , MD Z Alam1 , Noorahayu Yahya1 1. Bio-Environmental Research Unit, Department of Biotechnology Engineering, International Islamic University Malaysia, Jalan Gombak 50728, Malaysia. E-mail: [email protected]
2. Nanoscience and Nanotechnology Group, Department of Biotechnology Engineering, International Islamic University Malaysia, Jalan Gombak 507283, Malaysia 3. Department of Chemical Engineering, King Fahd University for Petroleum and Mineral, Saudi Arabia Received 01 February 2008; revised 12 September 2008; accepted 24 September 2008
Abstract The capability of carbon nanotubes (CNTs) to adsorb lead (Pb) in aqueous solution was investigated. Batch mode adsorption experiment was conducted to determine the eﬀects of pH, agitation speed, CNTs dosage and contact time. The removal of Pb(II) reached maximum value 85% or 83% at pH 5 or 40 mg/L of CNTs, respectively. Higher correlation coeﬃcients from Langmuir isotherm model indicates the strong adsorptions of Pb(II) on the surface of CNTs (adsorption capacity Xm = 102.04 mg/g). The results indicates that the highest percentage removal of Pb (96.03%) can be achieved at pH 5, 40 mg/L of CNTs, contact time 80 min, and agitation speed 50 r/min. Key words: lead removal; carbon nanotubes; kinetic modeling; adsorption DOI: 10.1016/S1001-0742(08)62305-0
Introduction Carbon nanotubes (CNTs), a new member of the carbon family, have good anion and cation adsorption materials for water treatment, as they exhibit exceptionally large speciﬁc surface area. In addition to the remarkable mechanical properties, their hollow and layered nanosized structures make them a good candidate as absorbers. Various technologies are currently employed in industry to deal with heavy metals such as chemical precipitation, reverse osmosis (Ahalya et al., 2007) and adsorption or ion exchange (Lu et al., 2007). In wastewater treatment, nanomaterials especially CNTs have been developed in remediation and end-of-pipe treatment technologies (Masciangioli and Zhang, 2003). Lead in wastewater comes mainly from the discharge of battery manufacturing, printing, dying and other industries (Li et al., 2002). Other major sources of lead in the environment include lead-based paint, household dust and food containers. Lead has been found to be acute toxic to human beings when present in high amounts in water. Studies have shown that young children, infants and pregnant women are particularly susceptible to unsafe lead levels (http://www.safe-drinking-water.com). For adults, increased levels of lead have been linked to high blood * Corresponding author: E-mail: [email protected]
pressure and damaged hearing. Drinking, eating, inhaling even at low level of lead can cause other serious health eﬀects. The aim was to study the removal of lead from synthetic water using CNTs by optimizing the process parameters to maximize the removal.
1 Materials and methods 1.1 Experimental The production of carbon nanotubes was conducted in two horizontal tubular reactors, using chemical vapor deposition (CVD) technique, which has been developed from Muataz (2005) technique. The horizontal reactors are a ceramic tube of 50 mm in diameter and 1200 mm in length and heated by silicon carbide heating element. The ferosine (C10 H10 Fe) catalyst of 100 mg was ﬁxed at the ﬁrst reaction chamber at 150°C for 10 min, while the second reaction chamber was used for the reaction with H2 O2 and for growth processes at 800°C for 30 min. Hydrogen was used as a reacting gas and the argon was used for ﬂushing the air from the system. Both of them were controlled by a ﬂow meter. 1.2 Batch mode adsorption experiment Experiments were conducted at 25°C to study the eﬀects of initial solution pH, CNTs dosage, contact time, and
Nassereldeen A Kabbashi et al.
agitation speed on the adsorption of Pb(II). Each test was conducted in volumetric ﬂask and the initial and ﬁnal concentration of Pb(II) were analyzed using atomic adsorption spectrometer (AAS) (AAnalyst 400, Elemer Precise, USA) at wavelengths of 283.3 nm for lead. The ﬁnal concentration of each study was use to determine the Pb(II) removal percentage. The run orders for complete batch mode adsorption experiment were determined using matrix analysis (Levine, 2001).
2 Results and discussion 2.1 Eﬀect of pH on the uptake of lead The diﬀerences in percentage removal indicate that the initial pH would play a vital role in Pb(II) removal as shown in Fig. 1, where the percentage uptake of Pb(II) varied at diﬀerent pH values (3–7). Previous study has stated that the adsorption of Pb(II) increases with an increase in solution pH from 3 to 7. This is because oxidation of CNTs with oxidized acid can introduce many functional groups such as hydroxyl, carbonyl and carboxyl on the surface of CNTs (Li et al., 2002). The decrease in percentage removal at pH 7 reﬂects a reduction of negative surface charge density on CNTs. Therefore, the presences of a negative charge on CNTs surface over the pH range were the main reason for Pb adsorption. H+ should be considered as competitive ones in ion-exchange processes and consequently, ion exchange of metals favored by high acidity, which should, however, be lower than the minimum acidity of precipitation. (M(H2 O) x )c+ + H2 O ←→ (M(H2 O) x - 1 (OH))(c - 1) + H3 O+ (1) Consequently, the above equilibrium (Reaction (1))
shifted to the left at lower acidity and more highly charged metal complexes are formed. This fact is beneﬁcial for the exchange. Therefore, very low adsorption of the metal takes place from highly acidic solutions (Inglezakias et al., 2007). The white crystal structure in the image was analyzed as Pb(II). This was supported by energy dispersive X-ray (EDX) analysis in Fig. 2, where CNTs at pH 5 obtained the highest peak. The distribution of Pb at pH 5 was the highest (10.91%) compared to pH 3 (0.45%), and pH 7 (1.74%). Therefore, it can be concluded that Pb(II) have been adsorbed on the surface of CNTs. The maximum adsorption can be achieved at pH 5 with removal percentage of 84.78% (Fig. 1). The result agreed with the result by Bismarck and Wuertz (1999), that acidic surface sites give a negative zeta-potential, whereas basic sites give a positive zetapotential. This implies that at low pH, a signiﬁcant amount of basic groups which are able to induce a positive surface charge, are present on the surface. 2.2 Eﬀect of agitation speed on the uptake of lead As shown in Fig. 3, the removal percentage of lead is decreasing as the speed increases. The removal of lead reach to 37.76% at 50 r/min, while at 150 r/min only 3.49% of Pb(II) was removed from the solution. It can be concluded that the eﬀects of agitation speed on the uptake of lead are not signiﬁcant for Pb(II) removal. As the speed increases, the suspension may not become homogeneous due to the rapid agitation. This will increase the boundary layer between the solid and liquid phase. Thus, the removal of Pb(II) could achieve maximum value at 50 r/min. 2.3 Eﬀect of CNTs dosage on the uptake of lead As shown in Fig. 4, the highest percentage removal (82.54%) occurred at high dosage (10 mg). The reason is that the high CNTs dosage provided more adsorption site for the attachment of Pb(II) and this accessibility greatly enhanced the adsorption of lead. EDX analysis was conducted to verify the eﬀect of dosage on the Pb(II) removal from aqueous solution (Fig. 5). It was observed that the high dosage of CNTs obtained a high peak. The Pb(II) distribution was 15.90% at 10 mg of CNTs compared to 1.74% at 5 mg. This veriﬁed Pb(II) have been adsorbed on the surface of CNTs.
Fig. 1 Eﬀect of pH on the uptake of lead. Conditions: contact time 20 min; adsorbent 20 mg/L; pH 3, 5, and 7.
Energy dispersive X-ray analysis of CNTs for pH 3 (a), 5 (b), and 7 (c).
Kinetic adsorption of application of carbon nanotubes for Pb(II) removal from aqueous solution
Fig. 3 Eﬀect of agitation speed on the uptake of lead. Conditions: contact time 120 min; adsorbent 40 mg/L; agitation speed 50, 100, and 150 r/min.
Fig. 4 Eﬀect of dosage on the uptake of lead. Conditions: adsorbent 20 and 40 mg/L; contact time 20–120 min.
2.4 Eﬀect of contact time on the uptake of lead The equilibrium time was measured from 20 to 120 min and the eﬀect of contact time is determined by plotting the percentage uptake of Pb(II) against contact time (Fig. 6). It was observed that the removal rate was very fast for the ﬁrst 40 min, but it gradually becomes slower until reached a maximum at 80 min. It was also detected that the percentage uptake of Pb(II) became saturated from 80 to 120 min. 2.5 Kinetics of adsorption The kinetics were investigated using the information obtained from the eﬀect of dosage (dry-weight basis) at 25°C at three diﬀerent time intervals up to 100 min. The pseudo second-order equation (Fig. 7) was used in this study to investigate the mechanism of adsorption of lead by the CNTs and the potential rate-controlling steps, such as mass transport and chemical reactions (Ray et al., 2005). The values of pseudo second-order rate constant k2 , the
Fig. 6 Eﬀect of contact time on the uptake of lead. Conditions: adsorbent 40 mg/L; pH 5; contact time 20 to 120 min.
Fig. 7 Pseudo second-order kinetics of Pb(II) using diﬀerent dosage of CNTs.
initial adsorption rate, h and the adsorption capacity (qe ) are presented in Table 1. The plot of t/qt versus time as in Fig. 7 for both dosage of CNTs yields high correlation coeﬃcients (R2 = 0.9888 (5 mg) and R2 = 0.9998 (10 mg)). The second order-rate constant obtained from this ﬁgure are 5.860 × 10−3 for CNTs dosage (5 mg) and 4.220 × 10−3 (g/(mg·min)) for CNTs dosage (10 mg). The second order rate constant indicates that higher dosage of adsorbent required less time to achieve initial adsorption of Pb(II) due to its greater surface area. The equilibrium adsorption capacity, qe obtained from the graph also implies that the higher dosage of adsorbent (qe =37.594 mg/g) is capable to uptake more adsorbate compared to the lower dosage (qe = 18.727 mg/g). This result indicates that the rate controlling steps in the adsorption process are chemisorptions, where interactions (chemical bonding) involved sharing or exchange of electrons between the adsorbate and the adsorbent (Ray et al., 2005). This proves that there are strong interactions between Pb and CNTs.
Fig. 5 EDX analysis of CNTs with diﬀerent dosages. (a) 5 mg; (b) 10 mg.
Nassereldeen A Kabbashi et al.
542 Table 1
Kinetic parameters for pseudo second-order model
h (m/ (g·min))
5.860 × 10−3 4.220 × 10−3
R2 0.9888 0.9998
was chosen for the development of regression analysis using the MINITAB analysis to determine the maximum removal of Pb(II) by CNT. The design characteristics which have been used to develop an optimization equation are as follows: full factorial, 2 replicates, 4 factors, 2 levels, 1 centre point.
2.6 Adsorption isotherm
2.8 Modeling for the removal of lead using CNTs
The Langmuir and Freundlich equations were used to describe the data derived from the adsorption of Pb(II) by CNTs over the entire parameters range studied. The adsorption capacity for Langmuir (Xm) was 102.04 mg/g and for Freundlich (n) was 8.945 mg/g, determined from the slope as seen in equilibrium curve (Fig. 8). Langmuir isotherm model shows better ﬁtting (R2 = 0.9966) with the experimental data compared to Freundlich isotherm (R2 = 0.622). This indicates the applicability of monolayer coverage of Pb(II) on the homogeneous surface of the adsorbent. It is also due to the fact that, CNTs have greater surface area for metal adsorption (Karthikeyan et al., 1996). The good correlation coeﬃcient of Langmuir isotherm also indicates that Pb(II) is strongly adsorbed to the surface of CNTs. Therefore, it is veriﬁed that CNTs have great potential to be a good adsorbent for the removal of Pb(II) in water treatment. The usage of CNTs gives higher adsorption capacity (102.04 mg/g) compared to other adsorbents such as Bacillus cereus (70.423 mg/g) (Ray et al., 2005), M. spicatum (46.69 mg/g) (Ahalya et al., 2007), Oat (18.97 mg/g) (Rios et al., 1999). This is due to the large surface area of CNTs that was oxidized at pH 5. At pH 5, the functional groups that were attached to the surface of CNTs were deprotonated, which contribute to an increase in the negative charges on CNTs surface. Therefore, this increased the ability of the adsorbent.
For lead removal, ﬁve factors, namely, pH (A), agitation speed (B), CNTs dosage (C) and contact time (D) were selected to optimize the lead removal RPb .
2.7 Modeling by statistical analysis The factors in the adsorption study were examined using the graphical analysis, the best two levels for each factor
Fig. 8 Adsorption isotherms model for Langmuir kinetic model (a) and Freundlich kinetic model (b).
RPb = (528 − 72.7A − 5.07B + 18.5C − 2.24D + 0.722 A × B − 4.00A × C + 0.385A × D− 0.419B × C + 0.0294 B × D + 0.0581C × D+ 0.0843A × B × C − 0.00603 A × B × D) × 100% (2) In order to search the optimum lead removal, experiments were designed based on central composite design. The second-order regression model relates to the lead removal with the independent variables of A, B, C, and D. The value of the adjusted determination of coeﬃcient was also very high (95.09%) to indicate a high signiﬁcance of the model (Akhnazaroza and Kefarov, 1982; Khuri and Cornell, 1987). The ANOVA of quadratic regression model demonstrated the model was highly signiﬁcant, as an evident from the Fisher’s F-test with a very low probability Table 2 Analysis of variance (ANOVA) for the second-order regression model Source
Degree of freedom
Sum of squares
Regression Residual error Total
12 19 31
33484.7 589.3 34074.0
Statistical analysis for evaluating the linear, quadratic, and interaction eﬀects
Standard error t-Value coeﬃcient
Constant pH (A) Agitation speed (B) CNTs dosage (C) Contact time (D) A×B A×C A×D B×C B×D C×D A×B×C A×B×D Analysis of variance Source Regression Residual error Total
528.49 –72.74 –5.068 18.512 –2.2405 0.7216 –3.995 0.3854 0.41927 0.02935 0.05813 0.08425 0.006029
83.02 13.57 1.044 7.667 0.9583 0.1717 1.245 0.1557 0.09582 0.01198 0.01969 0.01575 0.001969
0.000 0.000** 0.000** 0.026* 0.030* 0.000** 0.005** 0.023* 0.000** 0.024* 0.008** 0.000** 0.006**
DF 12 19 31
SS 33484.7 589.3 34074.0
MS 2790.4 31.0
6.37 –5.36 –4.85 2.41 –2.34 4.20 –3.21 2.48 –4.38 2.45 2.95 5.35 –3.06 F 89.96
R-Sq: R2 obtained from the adsorption study (R-Sq = 98.3%); R-Sq(adj): adjusted R2 variation in the adsorption capacity (R-Sq(adj) = 97.2%). * P < 0.05; ** P < 0.01.
Kinetic adsorption of application of carbon nanotubes for Pb(II) removal from aqueous solution Table 4
Comparison of various adsorbents and its percentage uptake of Pb(II)
Adsorbent pH Maize leaf Mountain laurel Common persimmon Eastern redbud Southern magnolia Activated carbon Clinoptilolite Bentonite Bacillus cereus M16 CNTs CNTs
Initial contact time (min)
4 3 6 5 5
45 45 30 40 40
Condition Agitation speed (r/min) 300
200 100 5500
value (Pmodel > F = 0.000) (Table 2). The coeﬃcient of determination, R2 that was obtained from this study is 0.983, which means 98.3% of the variation in adsorption capacity can be explained by the pH, CNTs dosage, and agitation speed and contact time. It was also noted that the adjusted R2 obtained from this study is 97.2% of the variation in the adsorption capacity (Table 3). This adjusted R2 is necessary when comparing two or more regression models that predict the same dependent variable but have diﬀerent number of explanatory variables (Levine et al., 2001). By this adjusted R2 , the best model can be identiﬁed. It can be concluded from this study that the most inﬂuential factors that contribute to the highest percentage removal of lead are pH, CNTs dosage and agitation speed in which the interactions of these factors contribute to the highest t-value and lowest p-value. Therefore, interactive eﬀects are important for optimization of lead removal rather than the single factor for a time method (Kumar and Satyanarayana, 2007). 2.9 Optimum conditions for the removal of Pb(II) using CNTs The highest predictive percentage removal is 96.03%. The parameters that contribute to these optimal conditions are pH 5, 10 mg dosage of CNTs in 250 mL Pb(II) solution, agitation speed at 50 r/min and contact time of 80 min. The control of carbon surface chemistry through the exclusive introduction of a certain surface group is a natural goal for the lead removal using carbon structures. It is highly challenging, as most methods give a surface covered with a mixture of acidic and basic groups. Moreover, the properties of each group are again dependent on its neighbors (Schlogl, 1999). Therefore, the deposition of metal particles is usually achieved through multistep and time-consuming procedures. 2.10 Comparative analysis of various adsorbents In comparison with the adsorption kinetics of the various adsorbents, it was concluded that most of the removal process occurred very fast within the ﬁrst 40 min. It can be concluded that the adsorption capability of the adsorbent is highly dependent on many factors such as surface functional groups, the speciﬁc surface area and the solution components (Table 4).
96 95.9 95.9 91.8 92.9 93.9 55 100 96 87.8 96.03
Adesola et al., 2006 Adeyiga et al., 2006
Dosage (mg/L) 10000 10000
20000 1800 500 40
Inglezakias et al., 2007 Ray et al., 2005 Li et al., 2002 This study
3 Conclusions The optimum pH is 5 in which gave 85% removal of Pb(II) from aqueous solution. The percentage uptake decreased with an increase in agitation speed from 50 to 150 r/min, in which 50 r/min gave 37.76% removal. The percent removal of Pb(II) was observed to be optimal for higher dosage of CNTs, in which 10 mg contribute to 82.54% removal of Pb(II). The Langmuir model ﬁtted best, in which the highest adsorption capacity is 102.04 mg/g. The eﬀect of contact time experiment indicated that higher fraction of the Pb(II) migrates from the bulk solution through the adsorbent boundary layer onto the active sites of the adsorbent. The overall adsorption rate demonstrated that the kinetics of the adsorption of Pb(II) on the CNTs was best described by pseudo second-order model. The results obtained from these analyses proved that this method of adsorption of Pb(II) using CNTs are promising for further development of water and wastewater treatment. Acknowledgments The authors are grateful to the Kulliyyah of Engineering (KOE) and Department of Biotechnology Engineering, IIUM for supporting and providing the laboratory facilities.
References Adesola N A, Babalola J O, Sanni R A, 2006. Biosorption of lead ions from aqueous solution solution by maize leaf. International Journal of Physics Science, 1(1): 23–32. Adeyiga A A, Liang H U, Greer T, 2006. Removal of metal ions from wastewater with natural wastes. Hampton University, Hampton. Ahalya N, Ramachandra T V, Kanamadi R D, 2007. Biosorption of heavy metals. http://www.ces.iisc.ernet.in/energy/water/ paper/biosorption/biosorption.htm, accessed November 10 2007. Akhnazaroza S, Kefarov V, 1982. Experiment Optimization in Chemistry and Chemical Engineering. Moscow: Mir Publishers. Augustine A A, Orike B D, Edidiong A D, 2007. Adsorption kinetics and modeling of Cu(II) ions sorption from aqueous solution by mercaptoacetic acid modiﬁed cassava wastes. Electronic Journal of Environmental, Agricultural and Food Chemistry, 6(4): 2221–2233.
Nassereldeen A Kabbashi et al.
Bismarck A, Wuertz C, 1999. Basic surface oxides on carbon ﬁbers. Journal Springer, 37: 1019–1025. http://www.nebguide.com. 2007. Safe Drinking Water: Lead, from. January 26, 2007. Inglezakias V J, Stylianou M A, Gkantzou D, Loizidou M D, 2007. Removal of Pb(II) from aqueous solutions by using clinoptilolite and benzoate as adsorbents. Desalination, 210: 248–256. Karthikeyan R S, Rakhsit S K, Baradarajan A, 1996. Optimization of batch fermentation conditions for dextran production. Journal of Bioprocess Engineering, 15(5): 247– 251. Khuri A I, Cornell J A, 1987. Response Surfaces: Design and Analysis. New York: Marcel Decker Inc. Kumar P, Satyanarayana T, 2007. Optimization of culture variables for improving glucoamylase production by alginateentrapped Thermomucor indicaeseudaticae using statistical methods. Bioresoure Technology, 98(6): 1252–1259. Levine D M, Ramsey P P, Smidt R K, 2001. Applied Statististics for Engineers and Scientist: Using Microsoft Excel & MINITAB. USA: Prentice Hall. Li Y H, Wang S G, Wei J Q, Zhang X F, Xu C L, Luan Z K, Wu D H, Wei B Q, 2002. Lead adsorption on carbon nanotubes. The Journal of Chemical Physics Letters, 35: 263–266.
Li Y H, Zhu Y, Zhao Y, Wu D, Luan Z, 2006. Diﬀerent morphologies of carbon nanotubes eﬀect on the lead removal from aqueous solution. Journal of Diamond and Related Materials, 15: 90–94. Lu L, Wang K, Zhao X S, 2007. Eﬀect of operation conditions on the removal of Pb2+ by microporous titanosilicate ETS10 in a ﬁxed bed column. Journal of Colloid and Interface Science, 305(2): 218–225. Masciangioli T, Zhang W X, 2003. Environmental technologies at the nanoscale. Journal of Environmental Science Technology, 102: 108–116. Muataz A A, Suleyman, A M, Ismail A F, 2005. Multi-walled carbon nanotubes/ natural rubber nanocomposite. Journal of Nanotechnology, 1(0106): 1–11. Ray L, Paul S, Bera D, Chattopadhyay P, 2005. Bioaccumulation of Pb(II) ions from aqueous solutions by Bacillus cereus. Journal for Hazardous Substance Research, 5(1): 1–21. Rios J V, Oberto B, Tiemann K J, Torresday J L G, 1999. Investigation of metal ion binding by agricultural by-products. Proceeding of the 1999 Conference on Hazardous Waste Research. 121–130. Schlogl R, 1999. Carbons. In: Preparation of Solid Catalysts (Ertl G, Knoezinger H, Weitkamp J, eds.). Weinheim: WileyVCH. 138–145.